** DUSAN STOSIC **

**NUMERICAL SIMULATIONS OF MAGNETIC SKYRMIONS IN **
**ATOMICALLY-THIN FERROMAGNETIC FILMS **

Universidade Federal de Pernambuco posgraduacao@cin.ufpe.br www.cin.ufpe.br/~posgraduacao

Recife 2018

**Numerical simulations of magnetic skyrmions in**

**atomically-thin ferromagnetic films**

Thesis presented to the Programa de Pós-graduação em Ciência da Computação of Centro de Informática of Universidade Federal de Pernambuco and the Doctoral Study Program of University of Antwerp as partial requirement to award the joint degree of Doctor in Computer Science and Physics.

### Advisor: Teresa Bernarda

### Luder-mir

### Joint Advisor:

### Milorad Vlado

### Miloševi´c

### Recife

### 2018

** **

Catalogação na fonte

Bibliotecária Monick Raquel Silvestre da S. Portes, CRB4-1217

S888n Stosic, Dusan

*Numerical * *simulations * *of * *magnetic * *skyrmions * *in * *atomically-thin *
*ferromagnetic films / Dusan Stosic. – 2018. *

149 f.: il., fig.

Orientadora: Teresa Bernarda Ludermir.

Tese (Doutorado) – Universidade Federal de Pernambuco. CIn, Ciência da Computação, Recife, 2018.

Inclui referências e apêndice.

1. Inteligência artificial. 2. Filmes ferromagnéticos. I. Ludermir, Teresa Bernarda (orientadora). II. Título.

006.3 CDD (23. ed.) UFPE- MEI 2018-105

**Dusan Stosic **

“**Numerical Simulations of Magnetic Skyrmions in Atomically-thin **
**Ferromagnetic Films'” **

Tese de Doutorado apresentada ao Programa

de Pós-Graduação em Ciência da

Computação da Universidade Federal de Pernambuco, como requisito parcial para a obtenção do título de Doutora em Ciência da Computação

Aprovado em: 02/05/2018.

______________________________________________

**Orientadora: Profa. Dra. Teresa Bernarda Ludermir **

**BANCA EXAMINADORA **

____________________________________________

Prof. Dr. Tsang Ing Ren Centro de Informática /UFPE

______________________________________________ Prof. Dr. Paulo Salgado Gomes de Mattos Neto

Centro de Informática / UFPE

_______________________________________________ Prof. Dr. Milan Lalic

Departamento de Física / UFS

_______________________________________________ Profa. Dra. Viviane Moraes de Oliveira

Departamento de Física / UFRPE

_______________________________________________ Prof. Dr. Pedro Hugo de Figueirêdo

I would like to express sincere gratitude to my advisers Prof. Teresa Ludermir and Prof. Milorad Miloševi´c for their continuous and unconditional support throughout my doctoral studies. I also gratefully acknowledge funding from the Conselho Na-tional de Desenvolvimento Científico e Tecnológico (CNPq, No. 140840/2016-8) re-ceived towards the doctoral work.

Moore’s Law has driven the electronics industry for the past half century. How-ever, the doubling of transistors about every two years is beginning to break down, owing to fundamental limits that arise as they approach the atomic length. As a re-sult, the search for new pathways for electronics has become crucial. Among po-tential candidates, the discovery of magnetic textures known as skyrmions has at-tracted considerable interest and attention in spintronic technology, which relies on both the electron charge and its spin. The unusual topological and particle-like be-havior launched skyrmions into the spotlight of scientific research. Topological pro-tected stability, nanoscale size, and low driving currents needed to move them make skyrmions promising candidates for future consumer nanoelectronics. Recent ad-vances in the field have provided all of the basic functions needed for carrying and processing information. In this thesis, we look to advance the current understanding of skyrmion physics, and explore their potential to replace conventional electronics technology. First, the fundamental properties and lifetimes of racetrack skyrmions at room temperature are investigated. We discover that skyrmions can easily collapse at the boundary in laterally finite systems, and propose ways to improve their stability for constrained geometries. Then, pinning of single skyrmions on atomic defects of distinct origins are studied. We reveal that the preferred pinning positions depend on the skyrmion size and type of defect being considered, and discuss applications where control of skyrmions by defects is of particular interest. Next, we explore other magnetic configurations that can compete with skyrmions when considering new ma-terials, and describe a previously unseen mechanism for collapse of skyrmions into cycloidal spin backgrounds. Finally, switching and interactions between skyrmions with distinct topologies are reported. We find that skyrmions transition to higher or lower topologies by absorbing a unit spin texture. The interactions between skyrmions of different topological charges can be attractive or repulsive, leading to the formation of arranged clusters. We conclude with a numerical library for simulating magnetic skyrmions in various scenarios.

A Lei de Moore tem impulsionado a indústria eletrônica no último meio século. No entanto, a duplicação de transistores a cada dois anos está começando a quebrar, devido aos limites fundamentais que surgem à medida que se aproximam a largura atômica. Como resultado a busca por novos caminhos para a eletrônica se tornou crucial. Entre os potenciais candidatos, a descoberta de texturas magnéticas conheci-das como skyrmions atraiu muito interesse e atenção na tecnologia spintrônica, que depende ambos da carga e do spin de elétrons. O comportamento topológico e de partículas lançou skyrmions no centro de atenção da pesquisa científica. Skyrmions são candidatos promissores para a futura nano eletrônica do consumidor devido a sua estabilidade topológica, tamanho em nano escala e baixas correntes necessárias para movê-los. Avanços recentes fornecem todas as funções básicas necessárias para transportar e processar informação baseada em skyrmions. Nesta tese, procuramos avançar o conhecimento atual da física de skyrmions e explorar seu potencial para substituir a tecnologia eletrônica convencional. Primeiro investigamos propriedades fundamentais de skyrmions e sua estabilidade em temperatura ambiente. Descob-rimos que skyrmions podem escapar pela borda em sistemas finitos e propomos maneiras de melhorar sua estabilidade para geometrias restritas. Depois estudamos como skyrmions ficam presos em defeitos atômicos de origens distintas. Mostramos que as suas posições dependem do tamanho e do tipo de defeito a ser considerado, e também discutimos aplicações em que o controle de skyrmions por defeitos é de interesse. Em seguida, exploramos outras configurações magnéticas que podem com-petir com os skyrmions quando novos materiais são considerados, e descrevemos um mecanismo inédito para o colapso de skyrmions em fundos de spin ciclóides. Final-mente, relatamos as comutações e interações entre skyrmions de topologias distintas. Descobrimos que skyrmions transacionam para topologias mais altas ou mais baixas pela absorção de uma textura de spin unitária. As interações entre skyrmions de difer-entes cargas topológicas podem ser atrativas ou repulsivas, formando agrupamentos arranjados. Concluímos com uma biblioteca numérica para simular skyrmions mag-néticos em vários cenários.

De wet van Moore heeft de elektronica-industrie de afgelopen halve eeuw ge-dreven. De verdubbeling van transistors om de twee jaar begint echter af te nemen, vanwege de fundamentele limieten die ontstaan als ze de atoomlengte naderen. Als gevolg hiervan is het zoeken naar nieuwe wegen voor elektronica cruciaal geworden. Onder potentiële kandidaten heeft de ontdekking van magnetische texturen die be-kend staan als skyrmions veel belangstelling en aandacht getrokken in spintronische technologie, die berust op zowel de elektronenlading als de spin. Het ongewone topo-logische en deeltjesachtige gedrag introduceerde skyrmions in de schijnwerpers van wetenschappelijk onderzoek. Topologisch beschermde stabiliteit, nanoschaalgrootte en laagstromende stromingen die nodig zijn om ze te verplaatsen, maken skyrmions veelbelovend voor toekomstige nano-elektronica voor de consument. Recente ontwik-kelingen in het veld hebben alle basisfuncties opgeleverd die nodig zijn voor het dragen en verwerken van informatie. In dit proefschrift doen we ons best om het hui-dige inzicht in de skyrmion-fysica te verbeteren en hun potentieel te verkennen om de conventionele elektronische technologie te vervangen. Eerst worden de fundamentele eigenschappen en levensduren van racetrack skyrmions bij kamertemperatuur onder-zocht. We ontdekken dat skyrmionen gemakkelijk kunnen instorten aan de grens in zijdelings eindige systemen, en manieren kunnen voorstellen om hun stabiliteit voor beperkte geometrieën te verbeteren. Vervolgens pinning van enkele skyrmionen op atomaire defecten van verschillende oorsprong worden bestudeerd. We onthullen dat de voorkeurspinposities afhankelijk zijn van de skyrmiongrootte en het type defect dat wordt overwogen, en bespreken toepassingen waarbij de beheersing van skyrmi-onen door defecten van bijzonder belang is. Vervolgens verkennen we andere magne-tische configuraties die kunnen concurreren met skyrmionen bij het overwegen van nieuwe materialen en beschrijven een tot nu toe onzichtbaar mechanisme voor het instorten van skyrmionen in cycloïdale spin-achtergronden. Ten slotte worden over-schakeling en interacties tussen skyrmionen met verschillende topologieën gerappor-teerd. We vinden dat skyrmionen overgaan naar hogere of lagere topologieën door een spinstructuur van een eenheid te absorberen. De interacties tussen skyrmionen van verschillende topologische ladingen kunnen aantrekkelijk of afstotend zijn, wat leidt tot de vorming van geordende clusters. We sluiten af met een numerieke bibli-otheek voor het simuleren van magnetische skyrmionen in verschillende scenario’s.

2D Two-dimensional

AFM Antiferromagnetic

Co Cobalt

CPU Central Processing Unit

DFT Density Functional Theory

DM Dzyaloshinsky-Moriya

DMI Dzyaloshinsky-Moriya Interaction

DW Domain Wall

eV Electron Volt

Fe Iron

FM Ferromagnetic

GNEB Geodesic Nudged Elastic Band

GPU Graphics Processing Unit

Ir Iridium

LL Landau-Lifshitz

LLG Landau-Lifshitz Gilbert

MC Monte Carlo

MEP Minimum Energy Path

ML Monolayer

MgO Magnesium Oxide

NEB Nudged Elastic Band

Pd Palladium

Pt Platinum

QM Quick-Min

SCy Spin Cycloid

SkX Skyrmion Lattice

SOC Spin-Orbit Coupling

SP Saddle Point

SP-STM Spin-Polarized Scanning Tunneling Microscopy

**1** **INTRODUCTION . . . .** **13**

**1.1** **Timeline** . . . **15**

**1.2** **Technologies** . . . **18**

1.2.1 Detection . . . 19

1.2.2 Writing and deleting . . . 19

1.2.3 Motion by currents . . . 21

1.2.4 Towards devices . . . 21

1.2.5 Lifetimes . . . 24

**1.3** **Motivation** . . . **25**

**1.4** **Organization** . . . **27**

**2** **THEORY AND NUMERICAL CONCEPTS . . . .** **28**

**2.1** **Skyrmions** . . . **28**

2.1.1 Spin structure . . . 28

2.1.2 Helicity and vorticity . . . 29

2.1.3 Topological protection . . . 30

**2.2** **Atomistic spin model** . . . **31**

2.2.1 Exchange interactions . . . 31

2.2.2 Magneto-crystalline anisotropy . . . 34

2.2.3 Externally applied fields . . . 34

2.2.4 Dipole-dipole interactions . . . 34

**2.3** **Features in the numerics** . . . **35**

2.3.1 Multi-scale modeling . . . 35

2.3.2 Beyond nearest neighbors . . . 36

2.3.3 Material inhomogeneities . . . 36

**2.4** **Spin dynamics** . . . **37**

2.4.1 Landau-Lifshitz-Gilbert equations . . . 37

2.4.2 Langevin dynamics . . . 39

2.4.3 Time integration . . . 39

**2.5** **Minimum energy paths** . . . **40**

2.5.1 The case of magnetic transitions . . . 40

2.5.2 Geodesic nudged elastic band . . . 41

2.5.3 Optimization procedure . . . 44

2.5.4 Climbing image . . . 45

**2.6** **Monte Carlo** . . . **46**

**3** **SKYRMIONS IN FEW-MONOLAYER FERROMAGNETIC FILMS** **49**
**3.1** **Introduction** . . . **49**

**3.2** **Stability of a skyrmion** . . . **51**

3.2.1 Three monolayers Co on Pt . . . 51

3.2.2 Three monolayers Co in a spin-orbit sandwich . . . 55

**4** **PINNING OF MAGNETIC SKYRMIONS . . . .** **67**

**4.1** **Introduction** . . . **67**

**4.2** **Pinning fundamentals** . . . **69**

4.2.1 Pinning on material defects . . . 69

4.2.2 Pinning in holes . . . 73

**4.3** **Employing the defects** . . . **75**

4.3.1 Controlled breathing of a skyrmion . . . 75

4.3.2 Skyrmion ratchet . . . 78

4.3.3 Skyrmion on the rails . . . 79

**5** **FROM SKYRMION LATTICES TO SPIN CYCLOIDS . . . .** **82**

**5.1** **Introduction** . . . **82**

**5.2** **Analyzing the transitions** . . . **84**

5.2.1 Path of minimum energy . . . 84

5.2.2 Topological knot . . . 86

**5.3** **Influencing the stability** . . . **90**

5.3.1 Dependence on magnetic field . . . 90

5.3.2 Dependence on material parameters . . . 92

5.3.3 Effective energy landscape . . . 94

**6** **HIGHER ORDER SKYRMIONS . . . .** **96**

**6.1** **Introduction** . . . **96**

**6.2** **Non-trivial properties** . . . **97**

**6.3** **Switching behavior** . . . **98**

6.3.1 Same charged particles . . . 98

6.3.2 Pairs of opposite charges . . . 100

6.3.3 Nature of transitions . . . 100

**6.4** **Interactions. . . 103**

6.4.1 Attractive and repulsive . . . 103

6.4.2 Formation of clusters . . . 103
**7** **NUMERICAL LIBRARY . . . 105**
**7.1** **Interface** **. . . 105**
**7.2** **Geometry** **. . . 106**
**7.3** **Material images** **. . . 108**
**7.4** **The Hamiltonian** **. . . 109**
**7.5** **Diffusion search** **. . . 110**
**7.6** **Minimization** **. . . 112**
**7.7** **Ansatz** **. . . 114**

7.7.1 For magnetic states . . . 114

7.7.2 For magnetic paths . . . 116

**7.8** **Dynamic spin clustering** **. . . 119**

**7.9** **Optimizations** **. . . 120**

7.11.2 Collapse of a single skyrmion . . . 124

7.11.3 Escape of racetrack skyrmion at boundary . . . 124

7.11.4 Pinning on a material defect . . . 126

7.11.5 Spin dynamics of skyrmion clusters . . . 127

**8** **SUMMARY AND OUTLOOK . . . 129**

**8.1** **Summary** **. . . 129**

**8.2** **Outlook** **. . . 131**

**REFERENCES . . . 133**

**1 INTRODUCTION**

Since the era of electronics began with the invention of the transistor in 1947 and silicon-based semiconductor technology, companies were trying to make their prod-ucts smaller. Transistors are widely used in modern electronics as building blocks of electronic circuits. As transistors get smaller, more of them can be packed on a chip, they also get faster and consume less electricity. For the past four decades, the electronics industry has been driven by Moore’s Law [1], which effectively suggests that electronic devices double in speed and capability about every two years. Indeed, every two years companies come up with new chips that have double the number of transistors for processing [2] or for memory [3] (see Fig. 1.1). However, the expo-nential growth envisioned by Moore does not come without a cost. From a feature size of 90 nm around 2004 to one of 10 nm today, considerable progress was made in processing and patterning technologies, as well as in nanotechnology. Modern chips are manufactured with billions of transistors, making it extremely challenging to keep up with the exponential scaling. The doubling has already started to slow down due to heat that is inevitably generated when more silicon circuitry is packed into a small area [4]. Moreover, some even more fundamental limits on the physics await. As the size of a transistor reaches to the 2-3 nanometer limit, where features are just 10 atoms across, quantum mechanical effects begin to take place due to the wavelike behavior of particles [5, 6]. Precisely, at that scale particles behave in strange ways, taking on more than one state at the same time and interacting with other particles that are very far away, that will make transistors hopelessly unreliable [2]. These issues ap-pear both on the processing and memory side, with little chances for solutions using current technology.

Figure 1.1 – Increase of the number of transistors per chip together with the increase of their clock speed, adapted from Ref. [2].

Figure 1.2 – Technology scaling options based on new paradigms and materials, adapted from Ref. [7].

For many years silicon was the only option for electronics. However, recent de-velopments in material-engineering and nanotechnology, as well as in other fields of science, have introduced new pathways for electronics (see Fig. 1.2). One possibility is to embrace a completely new paradigm like quantum computing [8, 9], which har-nesses quantum phenomena to process information in a novel and promising way, or neuromorphic computing [10, 11], which aims to mimic neurons in the brain, or even photonic computing [12], which use light instead of electricity for processing. But none of these alternative paradigms has left the laboratory, and many are believed to offer advantages only for specific applications, rather than for the everyday tasks of digital computing. A different approach is to stick with silicon, but configure it in entirely new ways. One popular option is to expand vertically by stacking many thin layers of silicon circuitry [2]. While this works for memory chips that consume power only when a memory element is accessed, which is not that often, microprocessor chips are more challenging as stacking layer after layer of hot circuits only makes the heat problem worse. Finally, one can stay in the digital realm, but look for materials that could be used for electronics as fast as their silicon counterparts while generating much less heat. There are many candidates, ranging from graphene [13] and other near 2D-like compounds [14], to organic electronic materials [15], based on organic molecules or polymers using chemical synthesis, to memristors [16], which couples the electrons with electrically charged atoms called ions.

Among the various potential candidates, spintronic materials [17], that rely not only on the electron charge but also on its spin to carry and process information, have attracted considerable interest and attention. The spotlight of this technology are skyrmions, topological spin textures that were recently discovered in magnetic materials. Skyrmions are promising candidates for future consumer nanoelectronics due to their topological protected stability, nanoscale size, and low driving currents needed to move them. Recent advances in the field have provided all of the basic functions needed for storing and processing information, which further highlights

their potential for future electronic applications [18]. In this thesis, we procure to advance the theoretical understanding of magnetic skyrmions in various situations, and explore their potential to replace conventional electronics technology.

**1.1**

**Timeline**

Since the 1950s, the problem of how to explain the presence of countable particles in continuous fields has been of interest [19]. Stable localized field configurations were searched to form a general field theory of elementary particles, but the majority of nonlinear field models were unable to predict them. As an exception, in 1961 Skyrme was able to describe nuclear particles as localized states called ‘skyrmions’ [20]. In quantum field theory, particles are wave-like excitations with finite lifetimes. Skyrme proposed to describe their stability by treating the particles as topological defects in a quantum vector field. These defects are characterized by a topological integer that cannot be changed through continuous deformation of the field, leading to the notion of “topological protection”. Interestingly, they have turned out to be relevant in condensed matter systems such as the quantum Hall system [21], liquid crystals [22], and Bose condensate [23]. Indeed, it was found that topologically protected particles can also appear in chiral magnets in the form of stable spin textures [24], referred to as magnetic skyrmions, the protagonist of this thesis.

For over a decade, theoretical predictions [27–30] of skyrmion excitations in con-densed matter systems with chiral interactions were made. Following these pioneer-ing theoretical works, a set of experiments in 2009 [26,31,32] established the existence of skyrmion phases in magnets. A key ingredient to their existence is the Dzyaloshin-sky–Moriya (DM) interaction [33, 34], which results from spin-orbit coupling (SOC) in a structure without inversion symmetry, for example, a chiral crystal structure or a surface. Extended lattices of magnetic skyrmions, as shown in Fig. 1.3, were first observed in B20-type bulk and thin film chiral magnets [35], such as MnSi [26],

Fe1−xCoxSi [36], FeGe [37, 38], or Mn1−xFexGe [39]. In B20 magnets, the chiral

inter-Figure 1.3 – (a) Crystal structure of MnSi with B20 cubic symmetry, retrieved from Ref. [25]. (b) Skyrmion crystal state imaged by Lorentz TEM with the superimposed spin orientation. (c) Phase diagram of MnSi as a function of temperature T and field B. Inset: Schematic of the skyrmion “A” phase, retrieved from Ref. [26].

### ( b )

### ( a )

### ( d )

### ( c )

Figure 1.4 – (a) Néel-type and (b) Bloch-type skyrmions, retrieved from Ref. [44]. (c) Lattice of skyrmions as observed by SP-STM in a monolayer of Fe grown on Ir(111). Colors indicate in-plane magnetization, retrieved from Ref. [45]. (d) Individual skyrmions observed by the same technique in a PdFe bilayer on Ir(111), where out-of-plane magnetization is color-coded from red for ‘up’ to blue for ‘down’ magnetization, retrieved from Ref. [46].

actions are induced from the lack of space-inversion symmetry in the atomic crys-tal, seen in Fig. 1.3(a), which creates weak SOC in the form of DM interactions. These interactions are ultimately responsible for the existence of skyrmion states. The skyrmion lattices can be moved by very small electrical currents and simulations have shown they are less hindered by defects [40]. However, this state only exists in a finite and narrow temperature region, labeled as the “A” phase in Fig. 1.3(c), which indicates that it can only be observed below room temperatures and in the presence of an external magnetic field. Fortunately, recent experiments have shown that robust skyrmion states can be achieved near or beyond room temperatures [41, 42] and for a wide range of fields [43].

Until then, skyrmion phases were restricted to bulk magnets with a particular chi-ral crystal symmetry, namely B20 compounds, greatly limiting the available systems that can be considered. Starting from 2011, skyrmions were also observed in ultra-thin magnetic films epitaxially grown on heavy metals, which are subject to large DM interactions (DMIs) induced by the breaking of inversion symmetry at the interface and to the strong SOC of the neighboring heavy metal. The Néel-like skyrmion states observed in ultrathin metallic films differ substantially from the Bloch-like skyrmions found in bulk materials, as illustrated in Fig. 1.4. The first investigated systems in this class were Fe monolayers on Ir(111), where a nanoscale skyrmion lattice was found to form the magnetic ground state by scanning tunnelling microscopy (STM) [47].

Figure 1.5 – (a) Asymmetric metallic multilayer made of several repetitions of a
tri-layer composed of a Co tri-layer (grey) sandwiched between two different
heavy metals, Pt (green) and Ir (blue). (b) Scanning transmission X-ray
microscopy (STXM) of skyrmions with sizes below 100 nm in Ir/Co/Pt
multilayers. (c) Skyrmion radius R plotted against the magnetic field
B for different DM couplings D. Figures are retrieved from Ref. [49].
(d) XMCD-photoemission electron microscopy image of a skyrmion in a
square dot patterned in a Pt/Co/MgO trilayer, indicated by the white
dashed line, retrieved from Ref. [50]. (e) Examples of stable spin
*struc-tures for 2 µm discs close to the Pt/Co/Ta sample used in experiments,*
retrieved from Ref. [51].

The large DM and weak exchange interactions for the Ir/Fe interface leads to Néel skyrmions which are forced on a square lattice with a period of only 1 nm by the four-spin interaction (see Fig. 1.4(c)), formed spontaneously even in zero external magnetic field. However, this skyrmion lattice cannot be driven into a different topo-logical state, and as result does not seem suited for exploring single skyrmions. In-stead, Romming [48] showed that adding an atomic Pd overlayer can push the system into a regime where skyrmion phases are observed at low field, but an applied field on the order of 1 T induces a transition to a ferromagnetic state embedding individual metastable skyrmions, shown in Fig. 1.4(d), that can be manipulated by spin-polarized currents in STM. For further increases of the magnetic field, the system undergoes a second transition into the saturated ferromagnetic phase.

So far, the nanoscale skyrmions in Fe monolayers and PdFe bilayers on Ir(111) could only be observed at low temperatures, typically 4 K, and high magnetic fields, typically 1.5 T. However, a prerequisite for their practical use is the ability to stabilize small individual skyrmions at room temperature and in near-zero applied fields. A promising path towards this goal can be achieved by increasing the thickness of the

transition metal film, by making use of interlayer exchange coupling, or by design-ing asymmetric multilayer structures [45]. This has been well demonstrated in series of publications in early 2016 for multilayer structures formed by stacking layers of magnetic and non-magnetic heavy thin metallic films [49–51]. For example, Ref. [49] showed that in metallic multilayers with Co layers sandwiched between two different heavy-metal layers, such as Ir and Pt illustrated in Fig. 1.5(a), the additive interfa-cial DM interactions are large enough to stabilize skyrmions below 100 nm in size at room temperature and in external fields of only a few tens of millitesla (see Fig. 1.5(b-c)). This results from a coupling of the skyrmions in successive Co layers, combined with the increase of the effective magnetic volume obtained by repeating the mag-netic layer vertically. Refs. [50] and [51] achieved similar sub-100 nm skyrmions at room temperature, shown in Fig. 1.5(d-e), by employing multilayers of Pt/Co/MgO and Pt/Co/Ta, respectively. Importantly, this type of multilayer can be fabricated by sputter deposition, which are standard technologies for industrial production [44].

Lastly, there is increasing interest in new classes of nanoscale topological spin textures in magnets, since they are expect to provide new means for electric control of magnetism. The relevant literature has been mostly focused on skyrmion textures that arise in materials with chiral interactions of the DM type. However, besides the DM interaction, chiral interactions can also arise from the four-spin interactions [47], which occurs due to electron hopping between four adjacent sites, and frustration in the isotropic exchange interactions [52]. The latter is particularly useful for the creation of various distinct skyrmion-like structures in magnets. Recently, it was dis-covered experimentally that a phase consisting of skyrmion and anti-skyrmion lattices can be stabilized in the triangular spin model with competing interactions [52]. Then, a rich phase diagram of an anisotropic frustrated magnet with frustrated skyrmions of arbitrary vorticity and helicity was investigated [53]. Simultaneously, a new form of particle-like state, composed of a smooth magnetization vector field and a mag-netic singularity, was found on the surface of bulk chiral magnets. Ref. [54] revealed a new class of skyrmion crystals, while Ref. [55] analyzed skyrmion and anti-skyrmion pair creation by spin-polarized currents. Other variants of skyrmion-like structures in frustrated magnetic materials have also been studied theoretically [56–58].

**1.2**

**Technologies**

Skyrmionics refers to the emerging technologies based on magnetic skyrmions in the fields of spintronics and nanoelectronics. Skyrmions can be used as information carriers in the next-generation information-processing devices due to their remarkable stability, extremely small size (down to a few nanometers), and very small current densities needed to displace them in nanostructures [40,59,60]. To realize the eventual commercialization of skyrmionics for future electronics, various challenges need to be solved such as creation and annihilation, detection, and manipulation of skyrmions. Here we discuss the technological advancements made in this context.

Figure 1.6 – (a) Differential tunnel conductance, dI/dU, map of two skyrmions with a profile along the arrow in inset. (b) dI/dU tunnel spectra in the skyrmion center (red) and in the FM background (black). Figures are adapted from Ref. [61]. (c) Schematic illustration of setup to measure topological Hall effect (top). Calculated topological Hall effect conductance as a func-tion of distance between skyrmion and Hall contacts (bottom), retrieved from [44, 62].

### 1.2.1

### Detection

In view of future skyrmionics, a key issue is the detection of individual nanoscale skyrmions. Several magneto-electric phenomena can be used towards this end. Op-erating a spin-polarized scanning tunneling microscopy (SP-STM) allows for direct real-space observation of complex non-collinear spin configurations. Specifically, in-dividual skyrmions were observed with atomic-scale spatial resolution using SP-STM imaging [46,48], where low tunneling currents and low bias voltages are typically cho-sen. Ref. [61] proposed a detection scheme that takes advantage of the non collinear magnetoresistance that arises. This magnetoresistance effect, called NCMR, is associ-ated with the large magnetization gradient observed in the presence of a skyrmion, illustrated in Fig. 1.6(a-b), and was used to detect skyrmions on a one-by-one basis. However, the NCMR depends on the highly non-collinear spin structure rather than on the topological properties of the skyrmion. A similar consideration holds for the longitudinal anisotropic magnetoresistance, or the anomalous Hall effect [63]. An-other approach for the efficient detection of skyrmions relies on the topological Hall effect [62], and is directly related to the topological properties of skyrmions. This ef-fect arises from the accumulated Berry phase which is proportional to the skyrmion number and creates an emergent magnetic field. Produced by the skyrmion, this emer-gent field leads to a measurable Hall voltage that allows a purely electrical detection of skyrmions [62], as shown in Fig. 1.6(c). While the topological Hall effect has been observed in bulk magnets, it remains to be reported at room temperature for metallic multilayers [44].

### 1.2.2

### Writing and deleting

Any application of future skyrmionics will require the ability to write and delete individual skyrmions. One possible route to achieve these goals is through current-induced effects. For example, Ref. [64] proposed creating skyrmions around an

ar-Figure 1.7 – (a) Snapshots of the creation of a skyrmion around a notch by current-induced spin transfer torque, adapted from Ref. [64]. (b) Schematic repre-sentation of a device for vertical spin injection through a magnetic tunnel junction, retrieved from Ref. [65]. (c) Nucleation of skyrmion bubbles by current-induced expansion of domains at the exit of a constriction, re-trieved from Ref. [66]. (d) Concept of skyrmion manipulation with local currents from an SP-STM probe tip, retrieved from Ref. [48]. (e) Deleting (left) and writing (right) skyrmions by local electric fields, retrieved from Ref. [67].

tificial notch by the action of the current-induced spin transfer torque, as shown in Fig. 1.7. To avoid the introduction of local defects, one can instead inject the spin-polarized current vertically through a magnetic tunnel junction (see Fig. 1.7), where the spin torques under the injection contact lead to the formation of a magnetic skyrmion [65]. This nucleation process was experimentally observed by injecting a current through a SP-STM in an FePd bilayer [48]. While originally introduced for the real-space observation of individual nanoscale skyrmions, by increasing the tunnel-ing current and the applied bias voltage the SP-STM can be used write and delete nanoscale skyrmions in a reproducible manner by local injection of spin-polarized electrons, as shown in Fig. 1.7. The energy of the injected electrons dictates the switch-ing between the skyrmion and ferromagnetic states, and the exerted spin-transfer torque provides a means to control the direction of switching [45]. An alternative approach involves the current-induced expansion of domains at the exit of a con-striction, seen in Fig. 1.7, which leads to the formation of micrometer-sized magnetic skyrmion bubbles [66]. Lastly, it has been demonstrated that nanoscale skyrmions can also be created and deleted by local electric fields [67], generated from a non-magnetic tip as shown in Fig. 1.7, where the polarity of the applied bias voltage provides a means to control the directionality of the switching, or skyrmion writing and deleting processes. This offers an interesting all-electric alternative to the

spin-transfer-torque-based switching by local spin-polarized current injection [45].

### 1.2.3

### Motion by currents

Skyrmions will be used for spintronic devices only if they can be moved or excited at low enough energy costs. Therefore, the motion of skyrmions is an active area of research, and its effect from currents has been studied since early experiments of bulk crystals. In 2010, Jonietz [59] first detected a current-induced rotation of the skyrmion lattice in the B20 MnSi crystal, while a direct observation of its current-induced motion in the flow regime in FeGe was reported later in 2012 [68]. Mean-while, Schultz [69] established a means to estimate the skyrmion velocity from the correlation between the current-induced motion of skyrmion lattices and the devia-tion of the Hall resistivity. Particularly, it was found that the current densities required

to move skyrmion lattices are very small, a few 106 Am−2, which is five or six orders

of magnitude smaller than those needed to move domain walls (DWs), of the order

1012 Am−2 [60]. This is due both because skyrmion lattices couple efficiently to the

current, and because they remain relatively unaffected by disorder [40, 59]. Further-more, the efficient current-driven motion can result from the skyrmion interaction with the edges of a nanostructure. In general, the motion of skyrmions consists of a longitudinal motion, along the direction of the current, and a transverse motion, often dubbed the skyrmion Hall effect, generated by gyrotropic forces that are related to the topology of the skyrmion [60]. As shown in Fig. 1.8(a), the skyrmion has both longitudinal and transverse velocities under an applied current, but the transverse disappears close to the edge due to its repulsive interaction. Moreover, the direction of the longitudinal motion depends both on the chirality of the skyrmion and on the sign of the spin Hall angle, while the deflection along the transverse direction de-pends on the polarization at the center of the skyrmion, up or down. At sufficiently high current densities, the skyrmion will collapse by going over the edge.

For the theory of current-induced motion of skyrmions, the Thiele equation [70] for describing the dynamics of magnetic solitons can be used:

**F**+**G**×**v**+* αDv*=0, (1.1)

**where F is the sum of the force exerted by the skyrmion Hall effect and the repulsive**
**force from the track edges, G is a gyrovector oriented along the out-of-plane direction,**
* D is the dissipative tensor, v is the skyrmion velocity, and α is the Gilbert damping*
coefficient. Everschor [71] used the Thiele equation to describe the skyrmion
dynam-ics induced by spin torque. Iwasaki [40] then compared predictions from the Thiele
equation with numerical simulations of a skyrmion lattice and a spin helix, or a series
of DWs. They found that the depinning currents are practically zero for skyrmions,
the Magnus force and the flexibility of skyrmions to avoid pinning centers induce a
weak influence from defects, and the skyrmion velocity increases linearly with the
current according to a universal slope, as seen in Fig. 1.8(b-c).

### 1.2.4

### Towards devices

Bringing skyrmionics into electronic devices offers unique opportunities for informa-tion and communicainforma-tions technologies. For example, the concept of racetrack

### mem-( b )

### ( c )

### ( a )

Figure 1.8 – (a) Motion of a skyrmion in a track as it bends the trajectory owing to repulsion by the edge and finally propagates along the edge. (b) Pinning of the current-induced motion of skyrmions by defects (triangular region of higher perpendicular anisotropy) in a 40-nm-wide nanotrack for dif-ferent notch depths and current densities. (c) Skyrmion velocity v as a function of current density j for in-plane currents. Figures are adapted from Ref. [65].

ory [72], in which a train of up and down magnetic domains is moved electrically along a magnetic track, could be extended to skyrmionics. Specifically, Refs. [65,73,74] showed that exploiting the solitonic character of skyrmions, the information can be encoded by a sequence of individual skyrmions in a magnetic track, illustrated in Fig. 1.9(a). Such tracks for skyrmions may be realized using lithographic techniques to fabricate magnetic stripes which are put in contact with high SOC materials, or they may be aligned by spatial modulations of strain fields, magnetic anisotropies or relevant magnetic interactions [45]. Their diameters can be reduced by decreas-ing the width of the track, as shown in Fig. 1.9(b). The spacdecreas-ing between neighbordecreas-ing skyrmions in a track can be of the order of magnitude of the skyrmion diameter (down to a few nanometers) [65, 75], and many such tracks can be stacked close to-gether. This means that a much higher information density can be expected with skyrmions as compared with domain walls in a racetrack memory [60, 76]. Moreover, because their motion is induced by spin torques, skyrmions can be guided in straight and curved tracks alike. Interestingly, the concept of skyrmion racetrack can be easily transformed and adapted to produce a nanoscale skyrmion transistor [77] by adding a field-induced gate in a given part of the track that allows or forbids the passage of a skyrmion, creating the equivalent of the on-off switch of a transistor.

The fact that a skyrmion behaves like a particle has motivated the application of skyrmionics to logic devices. Most of them rely on the conversion between a sin-gle skyrmion and a pair of DWs. This allows one to perform basic logic operations by duplicating or merging skyrmions through the design of specific nanostructures. Ref. [78] proposed logic gates AND and OR based on these concepts, which can be used as a first step to realize a complete logical architecture that replaces existing spin

Figure 1.9 – (a) Individual and train of skyrmions in a racetrack, retrieved from Ref. [65]. (b) Micromagnetic simulations showing that skyrmions are compressed in a track. (c) Dispersion relation for spin-wave propagation along a magnonic waveguide with and without skyrmions, with gaps in frequency due to periodicity of the skyrmion lattice. (d) Frequency spec-tra of skyrmions excitation modes for different DM interaction constants, D. Figures are adapted from Ref. [44].

logic devices [44]. The ability to create artificial periodic arrangements of skyrmions in one- or two-dimensional nanostructures can be used for skyrmionic magnonic crys-tals. The artificial lattices are used to periodically modulate the magnetization and hence control the propagation of spin waves inside them. Skyrmionic crystals on the nanoscale can then be envisaged, which is unthinkable for conventional magnonic crystals. Such crystals can be dynamically reconfigured simply by changing the di-ameter of the skyrmions, or the periodicity of the lattice, or even by erasing it [79, 80], see in Fig. 1.9(c). Another class of components for which skyrmionics can be used are nanoscale radio-frequency devices. For example, Ref. [81] proposed the skyrmion breathing modes of a skyrmion, induced by spin torques, can be used to generate a radio-frequency signal, as illustrated in Fig. 1.9(d). Being a localized soliton, the skyrmion is less sensitive to external perturbations and the resulting spin torque os-cillator will exhibit a more coherent dynamic. Finally, a skyrmionic microwave de-tector was investigated in Ref. [82], which relies on the conversion of the resonant excitation of the breathing mode into a d.c. mixed voltage. For an extensive review of

skyrmionic devices, see Ref. [18].

### 1.2.5

### Lifetimes

An important and often overlooked concept for the eventual commercialization of skyrmionics is the lifetime of a skyrmion state, which is one of the focuses of this the-sis. Since skyrmions represent metastable states, they have finite energy barriers that can be overcome by thermal fluctuations. The lifetime describes the length of time a skyrmion exists before an excitation in energy induces its collapse to another avail-able magnetic spin texture. The study on lifetimes of topological spin textures began when Bessarab [83] proposed a new method for characterizing their transitions in magnetic systems, based on minimum energy paths shown in Fig. 1.10(a). Rohart [84] was the first to study the stability of a single Néel skyrmion, revealing two distinct mechanisms for its collapse. However, it was later shown [85] and proven [86] that in fact only an isotropic shrinking of the skyrmion, or rotation of magnetic spins in the radial direction, represents a correct transition mechanism for Co monolayers on Pt. Moreover, the energy barriers for such transitions were found to be very small, on the order of tens of mili-electronvolts, meaning that single skyrmions can exist only for very short time scales, of nanoseconds, in ultrathin films. To make matters worse, Ref. [87] found that their stability drops drastically near the edges of a racetrack mem-ory, as illustrated in Fig. 1.10(b). However, it was later demonstrated [88], as part of the results of this thesis, that the lifetime of skyrmions at room temperatures can be extended from nanoseconds to seconds by increasing the DMI and designing non-trivial atomic structures along the edges, making skyrmions much more favorable for future racetrack memories. Similar findings for the FePd bilayer on Pt were made in Ref. [89]. Other works on racetrack memories studied their energy surfaces [90] and confinement effects [91].

The lifetimes of skyrmions can also be considered in other contexts. Ref. [92] iden-tified a new particle-like state, the chiral “bobber” shown in Fig. 1.10(c), and studied its stability in chiral magnets. Recently, the pinning of magnetic skyrmions on ever present material defects was analyzed, and their geometries exploited for the realiza-tion of practical devices [93]. The skyrmion stability was also analyzed against com-peting spin configurations [94]; both works are results of this thesis. Interestingly, von Malottki [95] demonstrated that exchange frustration can greatly enhance skyrmion stability, based on parameters from first-principles calculations. Wild [96], however, used Lorentz transmission electron microscopy to study the lifetime of skyrmions and found a substantial reduction by entropic effects, an extreme case of enthalpy-entropy compensation. Another contribution to the area is the study of other topo-logical spin textures. Bessarab [97] recently characterized the stability and lifetime of anti-ferromagnetic skyrmions, and found them to be feasible to observe in experi-ments. Skyrmions with topological numbers other than unity were first investigated in Ref. [95], where the collapse of an anti-skyrmion was analyzed. This was extended to transition mechanisms and interactions between skyrmions of different topological orders [98], as a result of this thesis.

Figure 1.10 – (a) Minimum energy path for a single spin system with initial path cho-sen to lie near a maximum (red) between the energy minima (blue), while converged path is shown in pink. Figure is retrieved from Ref. [83]. (b) Initial path (left) and minimum energy path (right) for collapse of a skyrmion at the edge of a racetrack, adapted from Ref. [87]. (c) Min-imum energy path from a Bloch skyrmion to a pair of chiral bubbles

to a single chiral bubble for two thicknesses, L1 and L2, retrieved from

Ref. [92].

**1.3**

**Motivation**

Skyrmions exhibit fascinating new properties that distinguish the spin texture from others. Their behavior mimics that of particles, which along with their topology, makes them useful objects in which to encode information. Even though concepts of topology are ubiquitous in several of the most exciting recent advances in condensed matter physics, such as high-temperature interfacial superconductivity, quantum Hall effect, or topological insulators, magnetic skyrmions remain the most promising can-didates for consumer nanoelectronics. Amazing advances have been made in the field, providing all the basic function needed for information storage and processing: writ-ing (nucleation of individual skyrmions), processwrit-ing (current-induced motion), and reading the information (electrical detection of single skyrmions). However, many of the findings are obtained only at low temperature and for skyrmion lattices, rather than for single skyrmions at room temperature. Another issue is the misuse of nu-merical simulations for describing certain physics involving magnetic skyrmions. For example, the thermal stability (or lifetime) of single skyrmions, which is vital for their practical use in devices, cannot be quantified using the continuous description of mag-netization assumed in micromagnetics, by far the most popular numerical choice in magnetism. Similar arguments hold true in regards to the behavior and stability of skyrmions around defects, as well as their interactions with one another. Possibly, the overarching problem involves either processes that take too long for direct sim-ulations, such as magnetic transitions that are rare events on the time scale of spin oscillations, or twisting of the spin texture in a way that cannot be described contin-uously. In these situations, one must resort to another set of numerical approaches to accurately describe the desired physics. One viable candidate is minimum

en-ergy paths combined with atomistic models of magnetism (this will be discussed in more detail in Chapter 2). Therefore, the purpose of this thesis is to advance the current understanding of skyrmion physics, as well as provide possible applications for skyrmionics, using the discussed methods. The present work is very important for the experimental realization of nanoelectronic devices based on skyrmions and can be divided into the following categories:

**I. Skyrmions in multilayers:** To date, DMI has been found in few bulk materials,

but can also be induced in atomically thin magnetic films in contact with surfaces with large SOC interactions. Recent experiments have reported that isolated magnetic skyrmions can be stabilized even near room temperature in few-atom thick mag-netic layers sandwiched between materials that provide asymmetric SOC. However, a proper analysis of the lifetimes of single skyrmions in such multilayers remains lack-ing. We therefore study the thermal stability of isolated skyrmions in ultrathin chiral magnetic structures composed of few monolayers, and try to find ways to improve their stability for con-strained geometries. This will be the topic of Chapter 3.

**II. Pinning on defects:** Pinning due to ever present material imperfections

cru-cially affects the mobility of skyrmions. Therefore, a proper understanding of how magnetic skyrmions pin to defects is necessary for the development and performance of skyrmionic devices. Existing works assume a phenomenological model for pinning (effective parabolic potentials) rather than a microscopically justified one. We revisit the pinning of a magnetic skyrmion by considering the minimum energy paths for transition from pinned to unpinned states, exploring linear and planar defect geometries that can be exploited to develop practical devices. The results are presented in Chapter 4.

**III. Competing spin backgrounds:** The stability of isolated skyrmions was

thor-oughly studied in ferromagnetic cobalt or iron based structures. However, other spin configurations can compete with skyrmions when considering novel magnetic mate-rials and substrates, and a proper understanding of how magnetic skyrmions transit to alternative non-trivial spin structures becomes crucial, both from a theoretical per-spective and for applications in devices. We explore transitions between skyrmion lattices and spin cycloids, and provide reflections on their thermal stability against competing transi-tion mechanisms. This will be discussed in Chapter 5.

**IV. Manipulations in topology:** The discovery of nontrivial topological particles

has brought about much innovation in modern matter physics. A great deal of at-tention is being placed on metastable states characterized by high thermodynamic stability, which are able to persist for long periods of time. Among them, magnetic skyrmions have been of particular interest since they are expected to provide the means for electric control of magnetism. Such nontrivial topological particles are rather desirable as they can bring richer physics, and may allow for more involved practical applications. Recently, skyrmions with topological numbers other than unity have been studied theoretically, but their stability and mechanisms for transition re-main elusive both in theory and in experiments. We therefore report on the theoretical discovery of switching mechanisms and interactions between skyrmions with distinct topolog-ical charges. This will be the topic of Chapter 6.

**1.4**

**Organization**

The thesis is organized as follows:

**In Chapter 2, we introduce theoretical concepts of magnetic skyrmions. We also**
introduce the numerical approaches for simulating the considered magnetic textures.
The concepts put forth will be used in the rest of the thesis.

**In Chapter 3, we investigate the behavior of isolated skyrmions in ultrathin chiral**
magnetic films composed of few-monolayers. The structures considered are similar
to those used for multilayers at room-temperature, and an approach to improve their
stability in racetrack memories is proposed. The results of this Chapter are published
in Ref. [88].

**In Chapter 4, the effect of defects on pinning of magnetic skyrmions is **
investi-gated. We show that different material inhomogeneities have different effects on the
skyrmion. Linear and planar defect geometries that can be used in practical
applica-tions are also explored. The results of this Chapter are published in Ref. [93].

**In Chapter 5, we reveal that other spin configurations can compete with skyrmions**
when considering new materials. We put forth a previously unknown transition
mech-anism from skyrmion lattices to spin cycloids. Furthermore, we show that the effective
stability of single skyrmions is lowered when all possible spin configurations are
con-sidered. The results of this Chapter are published in Ref. [94].

**In Chapter 6, the underlying switching mechanisms between skyrmions with **
dif-ferent topological numbers is investigated. We find that skyrmions with higher
topo-logical charges are more likely to transition into other topologies. The interactions
between skyrmions of different topological charges can be attractive or repulsive,
leading to the formation of arranged clusters or a sea of isolated spin textures. The
results of this Chapter are published in Ref. [98].

**In Chapter 7, we present an overview of the numerical library which was **
devel-oped along with this thesis. The library represents a culmination of the computational
effort made in each of the previous chapters. The focus is placed on the numerical
ap-proaches that were used, and examples on how to simulate some of the discussed
problems. The results of this Chapter are published in Ref. [99].

**In Chapter 8, we briefly summarize the results of this thesis and give closing**
remarks and discuss future outlook.

**2 THEORY AND NUMERICAL **

**CON-CEPTS**

The unusual topology and particle-like behavior launched skyrmions into the spot-light of scientific research. In this Chapter we will detail some of the theory behind magnetic skyrmions. We start by introducing their spin structure and the atomistic spin model, which proves to be an extremely useful tool for their description. We then discuss the multi-scale approach that allows us to simulate systems closer to experiment. We are interested in inhomogeneous material systems, which we model with spatially varying material parameters and beyond nearest neighbor interactions. Working with skyrmions requires special numerical techniques, so we present three popular approaches that deal with magnetic systems on the atomic scale.

**2.1**

**Skyrmions**

### 2.1.1

### Spin structure

Skyrmions can be either of the Néel-type or the Bloch-type, which correspond to dif-ferent symmetries of the interaction between spins, resulting in difdif-ferent directions of rotation [44]. For example, this can be due to the underlying crystal lattice [26,32,100] for Bloch skyrmion, or due to the presence of an interface [47, 48] for Néel skyrmions. In most systems, the spin structure of skyrmions is determined by the competition be-tween chiral interactions of the isotropic exchange and Dzyaloshinskii–Moriya (DM) type. Other possible candidates for stabilizing magnetic skyrmions include frustra-tion of isotropic exchange interacfrustra-tions [52], four-spin interacfrustra-tions [47], and

dipole-m i m z l a t t i c e s i t e 0 0 - 1 + 1 γ = 0 γ = π P t / C o P d / F e / I r + 1 a s p i n

Figure 2.1 – Single Néel skyrmion in a Pd/Fe/Ir (top) and a Pt/Co (bottom) nanos-tructure. The spins are represented by cones which are centered on lattice sites, separated by the atomic distance a. The resulting skyrmions have

*Figure 2.2 – Skyrmion structures with varying m and γ. The arrows indicate the *
di-rection of the in-plane spin component, and the brightness indicates the
normal component to the plane, with white denoting the up direction
and black the down direction. Figure retrieved from Ref. [35].

dipole interactions. The latter is responsible for magnetic bubbles, but they would not have the defined chirality found in skyrmions [24, 60]. The size and shape of the skyrmion can be manipulated by the geometry of the system and external magnetic fields [76, 101].

The focus of this thesis is on Néel skyrmions, which consist of atomic spins ar-ranged in near two-dimensional magnetic structures, as illustrated in Fig. 2.1. On the atomic level, the structure contains spin orientations localized on atomic sites, sepa-rated by the lattice constant a. The lattice constant is the distance between atoms and depends on the magnetic material being considered. The spin at the skyrmion center (or core) points along an out-of-plane direction, while spins at the perimeter point in the opposite direction. The magnetization rotates radially from the skyrmion center to the perimeter, where the sense of rotation is set by the chirality (or equivalently, the helicity) of the skyrmion. We can determine the direction of the skyrmion by the orientation of the center spin, and the size from the spin orientations in the same half-plane as its direction.

### 2.1.2

### Helicity and vorticity

Skyrmions can be defined by the Pontryagin number Q (or topological number),

**which is a measure of the winding of the normalized local magnetization, ˆm**(**r**). In

two dimensions, the topological number can be mathematically described by

Q= 1
*4π*
Z
**ˆ**
**m**(**r**) ·
**∂ ˆ****m**(**r**)
*∂x* ×
**∂ ˆ****m**(**r**)
*∂y*
dxdy, (2.1)

**as the integral of the solid angle, 4π, and counts how many times ˆ****m**(**r**) = **mˆ**(x, y)

wraps the unit sphere [35, 102, 103]. Using the symmetry of the skyrmion, we can

represent the spins in the spherical variables Θ and Φ as

**ˆ**

S k y r m i o n s t a t e E n e r g y b a r r i e r O t h e r m a g n e t i c s t a t e T h e r m a l a c t i v a t i o n

Figure 2.3 – Artistic sketch of a metastable skyrmion being thermally activated and collapsing into another magnetic state.

with

Φ =*mφ*+*γ*, (2.3)

*where φ is the azimuthal angle (0* ≤ *φ* ≤ *2π) and γ is the helicity. The *

vortic-ity m determines the skyrmion number as Q = m. Special values of the helicity

*(γ* = *0, π/2, π, 3π/2) play important roles [56], they also determine the chirality of*

*the skyrmion. For Néel skyrmions the helicity is either γ* = *0 or γ* = *π* and

deter-mines whether the in-plane spins are oriented inward or outward (see Fig. 2.1), while

*Bloch skyrmions have helicity of γ*±*π*/2 which defines a clockwise or

counterclock-wise rotation of the in-plane spins. Different helicities are obtained for different DM

interactions. We may index a skyrmion as(*Q, γ*) with the use of the topological

num-ber and the helicity. Fig. 2.2 illustrates various skyrmion structures corresponding to

vorticity m = ±*1, and helicity γ* = 0, ±*π/2, π. Note that Q reverses sign when all*

**the directions of the magnetic moments are reversed, ˆm**→ −**m, and the configurationˆ**

can be called an “anti-skyrmion”.

### 2.1.3

### Topological protection

A question studied in many fields of science is the lifetime of metastable states. Ther-mal activation across energy barriers governs the lifetime of memory elements in electronics and the transport of ions and electrons in disordered media [96]. Often, these processes are controlled by the activation energy. Special attention is drawn to systems which are able to persist in a particular metastable state for an unbounded or noticeably long time. One prominent example, and the focus of these thesis, are skyrmions induced in magnetic materials with chiral interactions. Particularly, the non-trivial topology of skyrmions plays a crucial role in their stability [35, 84]. In the continuous limit, the topology gives rise to a topological barrier that protects the skyrmion from other competing spin configurations, such as ferromagnetic (FM) and cycloidal (helical or conical) orders [43], as the spin configuration cannot be twisted continuously to result in a magnetic configuration with a different topology. This can also be interpreted as the fact that a Bloch point has to appear, resulting in an infinite exchange energy contribution. However, in real materials the system is discrete with

magnetic moments localized on atoms, which results in finite energy or topological barriers that can be surpassed by thermal fluctuations, as illustrated in Fig. 2.3.

Owing to their topological protection, skyrmions are highly stable [104], but only in applied field and at low temperature, which limits their use as individual particles in devices. Therefore, understanding the extent of topological protection in magnetic skyrmions, as well as finding ways to preserve their stability, remains crucial. These concepts are addressed in this thesis.

**2.2**

**Atomistic spin model**

While quantum mechanical in nature, magnetic materials are heavily influenced by thermal effects that are often difficult to describe using standard approaches from quantum theory. Therefore, models of magnetic materials should combine their quan-tum mechanical characteristics with thermodynamic formalism, for example, using atomistic spin models. The physical basis of atomistic spin models is the localization of unpaired electrons to atomic sites, where atoms are treated as possessing localized magnetic moments. This assumption has been proven valid for ferromagnets based on first-principles calculations [105]. Atomistic models of magnetic materials origi-nated with Ising in 1925, as the first model of the behavior in a ferromagnet [106]. However, the forced quantization of atomic moments to one of two allowed states limits the uses of the Ising model in real materials, e.g., the anisotropy is infinite. A natural extension is to take a continuous description of the spin direction in three dimensions [107], which corresponds to the Heisenberg model. Stanley further gen-eralized the dimensionality of spins in the n-vector model [108], which reduces to the

Heisenberg model for n = 3. In some ways the classical spin model is analogous to

Molecular Dynamics, where the energy of the system is determined from quantum mechanics, but the time evolution and thermodynamics are treated classically [109].

The extended Heisenberg spin model describes the essential physics of a magnetic material at the atomic level, and is formed from a summation of energy contributions given by a Hamiltonian of the form

H = Hexc+ Hani+ Happ+ Hdip, (2.4)

* each of which describes the interaction between an atomic spin moment, µ*i, and

neighboring moments or external magnetic fields. Note that one can introduce a three

**dimensional unit vector, ˆm**i = * µ*i/|

*i|, describing the direction of the effective*

**µ*** mag-netic moment, µ*i, localized on atomic sites. Each of the individual contributions to

the Hamiltonian Hare described in detail below.

### 2.2.1

### Exchange interactions

As two identical particles are localized close to each other, their wavefunctions can overlap yielding the exchange interaction. The effect is due to the wavefunction of indistinguishable particles being subject to exchange symmetry, and the Pauli exclu-sion principle [110], which governs the orientation of electron spins in overlapping

### A F M

### F M

### m

_{i + 1}

### m

_{i + 2}

### m

_{i + 3}

### m

_{i}

Figure 2.4 – One-dimensional sketch to illustrate the effect of nearest neighbor isotropic and antisymmetric exchange interactions in FM (upper panel) and AFM (lower panel) materials.

exchange Hamiltonian

Hexc = −1

2

### ∑

_{ij}

**mˆ**iJij

**mˆ**j, (2.5)

in which the sum is taken over the exchange Hamiltonians for all the i, j pairs of the

system of interacting atomic moments. The tensorial exchange coupling,J_{ij}, is a 3×3

matrix of the form

J_{ij} =
J_{ij}xx J_{ij}xy J_{ij}xz
J_{ij}yx J_{ij}yy J_{ij}yz
J_{ij}zx J_{ij}zy J_{ij}zz
, (2.6)

where its elements can be denoted by J_{ij}*αβ* *and α, β* = x, y, z. The matrix describes the

exchange interaction between atomic sites i and j, and can be decomposed into three terms [111]:

J_{ij} = JijI + JijS+ JijA. (2.7)

I is the identity matrix and Jij represents the isotropic exchange interaction

Jij = 1

3Tr(Jij), (2.8)

which corresponds to the classical Heisenberg exchange. For ferromagnetic (FM)

ma-terials the exchange energy favors neighboring spins that align in parallel, or Jij >0,

and for antiferromagnetic (AFM) materials the interaction prefers the spins to align

anti-parallel, or Jij < 0, as shown in Fig. 2.4. This is by far the dominating term in

the Hamiltonian, and can be an order of magnitude larger than the next largest

con-tribution. The second term, JS

ij, corresponds to the traceless symmetric anisotropic

exchange coupling [112, 113]

J_{ij}S = 1

2(Jij+ J

T

### m

2### m

_{1}

### m

_{2}

### m

1### D

1 2### ( b )

### ( a )

_{D}

1 2
**Figure 2.5 – Schematic of DM interaction, D**12, induced by (a) the indirect exchange of

**the triangle composed of two atomic spins, ˆm**1**and ˆm**2, and an atom with

a strong SOC, and (b) at the interface between a ferromagnetic metal (grey) and a metal with a strong SOC (blue) (right panel). Figure was adapted from Ref. [60].

whereJT

ij is the transpose of the exchange tensor. This is also known as the anisotropic

exchange or two-site magnetic anisotropy. Lastly, the third term is the antisymmetric exchange interaction

J_{ij}A = 1

2(Jij− J

T

ij). (2.10)

The antisymmetric part represents the Dzyaloshinsky-Moriya interaction (DMI) [33, 34]

**ˆ**

**m**iJijA**mˆ**j =**D**ij· (**mˆ**i×**mˆ**j), (2.11)

**where D**ij is the Dzyaloshinsky-Moriya (DM) vector defined as

D_{ij}x = 1
2(J
yz
ij −J
zy
ij ), D
y
ij =
1
2(J
xz
ij −Jijzx), Dzij =
1
2(J
xy
ij −J
yx
ij ), (2.12)

arising from a three-site indirect exchange mechanism that couples two atomic spins to a neighbor atom with large spin-orbit coupling [114] (see Fig. 2.5). For atomically-thin ferromagnetic films considered in this thesis, the DMI is interfacial and can be

**written as D**ij = Dij· (**ˆz**×**uˆ**ij) **[48], where ˆz and ˆu**ij are unit vectors perpendicular to

the interface in the direction of the magnetic layer and pointing from site i to site j, re-spectively. The DM interaction lowers or increases the energy of the spins depending

**on whether the rotation from ˆm**i **to ˆm**j **around D**ij is in the clockwise or in the

anti-clockwise direction. For Dij >**0 the DMI favors anticlockwise rotations from ˆm**i**to ˆm**j,

while for Dij <**0 the interaction prefers clockwise rotations [47, 48]. If ˆm**i **and ˆm**j are

initially parallel, a strong DMI compared with the symmetric exchange interaction,

Jij**, will introduce a relative tilt around D**ij. This tilt is responsible for the formation

of magnetic skyrmions. We can then rewrite the exchange Hamiltonian as a func-tion of the isotropic, symmetric anisotropic, and antisymmetric (or DM) exchanges as

follows: Hexc = −1 2

### ∑

_{ij}

**mˆ**i(JijI + J S ij + JijA)

**mˆ**j (2.13) = −1 2

### ∑

_{ij}Jij(

**mˆ**i·

**mˆ**j) − 1 2

### ∑

_{ij}

**mˆ**iJ S ij

**mˆ**j−1 2

### ∑

_{ij}

**D**ij· (

**mˆ**i×

**mˆ**j) (2.14) = H

_{iso}+ Hsym+ HDM. (2.15)

### 2.2.2

### Magneto-crystalline anisotropy

The thermal stability of a magnetic material is dictated by the anisotropy, or the
ten-dency for atomic moments to align along a preferred spatial direction. While there are
different physical origins for anisotropy, the most important is the magneto-crystalline
anisotropy arising from the interaction of atomic spin orbitals with the local crystal
environment [115]. The simplest form of anisotropy is uniaxial, where the magnetic
**moments prefer to align along a single axis, ˆe. Uniaxial anisotropy exists where the**
crystal lattice is distorted along a single axis. For example, in ultrathin magnetic films
the anisotropy is normal to the surface. The uniaxial anisotropy Hamiltonian is given
by

Hani = −

### ∑

i

Ki(**mˆ**i· **ˆe**)2, (2.16)

where Ki is the anisotropic energy per atom i. Other forms of anisotropy include the

cubic anisotropy which appears in materials with cubic crystal structures, and the two-site anisotropy which originates from the interaction of neighboring spins.

### 2.2.3

### Externally applied fields

**Many magnetic problems consist of interactions with external applied fields, H**app.

External fields can arise in many ways, such as from an electric current or a nearby magnetic material. They play a crucial role in stabilizing nanoscale skyrmions in near two dimensional magnetic films. In an external field, magnetic moments will experi-ence a torque proportional to the angle between the field and the spin direction, as well as the field strength. The applied field energy is given by

Happ= −

### ∑

i

* µ*i·

**H**app, (2.17)

* where µ*iis the effective magnetic moment localized on atomic site i, as defined earlier.

This term favors a parallel alignment of the spins along the field direction, moving the system towards a ferromagnetic state for increasing values of the field.

### 2.2.4

### Dipole-dipole interactions

From electrodynamics, magnetostatic (or dipolar) interactions refer to the direct in-teraction between magnetic dipoles, or atomic spin moments. Thus, the magnetized body will have a certain dipolar field opposing the overall magnetization. This dipolar

field depends on the size and shape of the magnetic body, and on the separation of individual moments. In the point-dipole approximation, the Hamiltonian for dipole-dipole interactions is given by

H_{dip}= −*µ*0

*8π*

### ∑

_{ij}

3(* µ*i·

**ˆr**ij)(

*j·*

**µ****ˆr**ij) −

*i·*

**µ***j*

**µ**r3_{ij} , (2.18)

*which sums over all moment pairs, where µ*0 **is the permeability of free space, ˆr**ij is

the unit position vector between sites i and j, and rij is the distance between sites i

and j.

**2.3**

**Features in the numerics**

### 2.3.1

### Multi-scale modeling

Magnetism has a quantum origin with systems characterized by atomic magnetic mo-ments, the exchange interaction, and spin-orbit coupling, to name a few. These are the province of ab initio models, but long simulation times limits the problem size to several hundred atoms, making a study of macroscopic systems from first principles intractable. In addition, magnetic materials are heavily influenced by thermal effects which are typically difficult to incorporate into standard density functional theory approaches. Therefore, models of magnetic materials should combine quantum me-chanical properties with a robust thermodynamic formalism [109].

Density functional theory (DFT) calculations rely on the Hohenberg–Kohn–Sham
theory [116], which states that the total energy of a system can be described by the
*electron density, ρ. In practice, both the electron and spin density are used in the total*
energy expression for spin polarized systems [117]. DFT can calculate a wide range
of properties including lattice constants, localized spin moments, magnetic ground
states and effective anisotropy. Standard software packages such as VASP [118] and
FLEUR [119] make such calculations readily accessible. They provide detailed insight
into magnetic properties that can be used as input into atomistic models.

In this situation, multiscale modeling can provide a proper description by using the results from ab initio calculations (on a system with a small size) to provide the magnetic parameters which will be included in the atomistic simulations. A signifi-cant capability of the atomistic spin model is that magnetic properties calculated at the electronic level can often be mapped onto a Heisenberg spin model with effec-tive local moments. This multiscale electronic and atomistic approach treats magnetic materials at the natural atomic scale and avoids the continuum approximations of micromagnetics. However, one can also calculate effective parameters for larger scale micromagnetic simulations [120, 121]. The atomistic model can interface directly with micromagnetism by calculating interface properties at the atomic level, while treat-ing the bulk of the material with a micromagnetic description [122]. Such approaches have become popular in simulating magnetic skyrmions [123, 124].